TUNABLE MULTI-CHANNEL FILTERING USING 1-D PHOTONIC QUANTUM WELL STRUCTURES

B. Suthar* and A. Bhargava

Nanophysics Laboratory, Department of Physics, Govt. Dungar College, Bikaner-334001, India

Abstract—In the present study, we show that it is possible to
achieve multi-channel filters in one-dimensional photonic crystals
using photonic quantum well structures. The photonic quantum
well structure consists of different 1-D photonic structures. We use
(AB)_{8}/C* _{n}*/(BA)

_{8}structure, where A, B and C are different materials. The number of defect layers (C) can be utilized to tune the multi-channel filtering. The filter range can be tuned for desired wavelength with the change in angle of incidence for multi-channel filtering. 1. INTRODUCTION

During the last two decades, studies on photonic crystals (PCs) have drawn the interest of many researchers as the propagation of electromagnetic waves can be hugely modified by such structures [1, 2]. PCs are periodic array(s) of dielectric materials, generally, exhibiting characteristic electromagnetic stop bands known as photonic band gaps (PBGs). That is, the PCs can prohibit the propagation of electromagnetic waves whose frequencies lie within the PBGs. One-dimensional PC structures have many interesting applications such as dielectric reflecting mirrors, low-loss waveguides, optical switches, filters, optical limiters etc. It has been demonstrated theoretically and experimentally that specifically designed one-dimensional PCs exhibit absolute omnidirectional PBGs [3–10, 11].

Recently, tunable photonic filters [12–14] have attracted wide
attention due to their applications in optical communication and
ultra-fast optical processing. The quantity of information carried
by an *N* channel filter is *N* times that of a single channel filter.
Both semiconductor [15–17] and metal [18–20] quantum well (QW)

structures have attracted tremendous attention in fundamental studies as well as possible technological applications. Thus, it is expected that their photonic counterparts, photonic quantum well (PQW) structure, are also attractive materials for intensive research [21–22]. Qiao et al. [22] proposed a kind of PQW structure by assembling different photonic crystals (PCs) with positive-index materials (PIMs). Through these structures, the photonic bandgaps (PBGs) can be enlarged effectively, and narrow multichannel filters can be obtained when the constituent PBGs are designed properly [23, 24]. For these structures, however, the resonance modes as well as the PBGs vary noticeably with different incident angles and polarizations.

In the present work, we show theoretically that it is possible to achieve multi-channel filters in 1-D photonic crystal using photonic quantum well structures. These multi-channel filters depend on the defects and the angle of incident light.

2. THEORETICAL MODELS

The multilayered structure consists of alternate layers of high and low
refractive indices along the *x*-axis and placed between semi-infinite
media of refractive indices*ni* (refractive index of the incident medium)
and *ns* (refractive index of the substrate), as shown in Figure 1.

Applying the transfer matrix method (TMM), the characteristic matrices for the TE and TM waves have the form [25, 26]

*Mj* =
"

cos*βj* *−i·*sin_{qj}βj

*−iqj*sin*βj* cos*βj*
#

(1)
where coefficients *qj* = *nj*cos*θj*, (*j* = 1, 2) for the TE polarization

and coefficients *q _{j}* = cos

*θ*for the TM polarization,

_{j}/n_{j}*β*= (2

_{j}*π/λ*)

*n*cos

_{j}d_{j}*θ*,

_{j}*θ*is the ray angle inside the layer of refractive index

_{j}*n _{j}* and

*λ*is the wavelength of light in the medium of incidence. The total characteristics matrix for the

*N*periods of the structure is given by

*M* = (*Mj*)*N* =
·

*M*11 *M*12
*M*21 *M*22

¸

(2) The transmission coefficient of the structure for the TE and TM polarizations are given by

*t*= 2*qi*

(*M*_{11}+*q _{s}M*

_{12})

*q*+ (

_{i}*M*

_{21}+

*q*

_{s}M_{22}) (3) where coefficients

*qi,s*=

*ni,s*cos

*θj,s*for the TE wave and coefficients

*qi,s* = cos*θj,s/ni,s* for the TM wave, where the subscripts *i*, *j* and *s*
correspond to the quantities in the incident medium, periodic medium
of photonic crystal and substrate respectively. The transmission of the
structure is given by

*T* =*|t|*2 (4)

The schematic representation of the proposed structure is shown in
Figure 2. We consider a PQW structure having the following sequence
— (AB)8/C*n*/(BA)8. For AB stack, we choose the thicknesses*a*and*b*

for A and B materials, respectively. The thickness of the defect layer
C is taken as*d*. The proposed structure leads to conventional PC for
defect layer C as A in the present structure.

3. RESULTS AND DISCUSSION

In this section, numerical calculations on the transmission properties
of the one-dimensional photonic crystals using Equation (4) have been
presented. In the present work, we use (AB)_{8}/(C)* _{n}*/(BA)

_{8}structure, where (AB)

_{8}is the periodic multilayered structure consists of eight sub-layers of AB and (C)

*consist of n sub-layers of C. For AB stack, we choose the material of layer A as TiO2 and the material of layer*

_{n}B as SiO2 having refractive indices 2.41 and 1.5 respectively. The

incident medium is taken as air while the substrate is taken as glass.
The substrate has been used to define the actual coupling of photonic
filter device with other devices as per requirement. The thicknesses of
the alternate layers are taken as*a*= 182 nm and *b*= 291 nm according
to the quarter wave stack condition*a*=*λc/*4*n*1 and *b*=*λc/*4*n*2, while
*λc*= 1750 nm is the critical wavelength which is the mid-wavelength of
the wavelength range considered in our numerical computation. While

(a)

(b)

(c)

(d)

(e)

(f)

Figure 3. Transmission of PQW structure (AB)8C(BA)8, for TE

mode with angle of incidence (a) *θ* = 0*◦*_{, (b)} _{θ}_{= 45}*◦*_{, (c)} _{θ}_{= 80}*◦*
and for TM mode with angle of incidence (d) *θ*= 0*◦*_{, (e)} _{θ}_{= 45}*◦*_{, (f)}

(a)

(b)

(c)

(d)

(e)

(f)

Figure 4. Transmission of PQW structure (AB)8C2(BA)8, for TE

mode with angle of incidence (a) *θ* = 0*◦*, (b) *θ* = 45*◦*, (c) *θ* = 80*◦*
and for TM mode with angle of incidence (d) *θ*= 0*◦*_{, (e)} _{θ}_{= 45}*◦*_{, (f)}

*θ*= 80*◦*_{.}

for the defect layers C, we choose the material of layer C same as layer
A (TiO2) with the thickness of layer taken as *d* = 450 nm. Here, all

the regions are assumed to be linear, homogeneous and non-absorbing.
Also, the refractive indices of both the materials are considered to
be constant for incident wavelength region. The defect stack C*n* is a
cavity stack whose spectral response overlaps with the spectrum of the
primary stack. The defect C*n* layers play a role of a refractive index
well or cavity depending on the wavelength of electromagnetic waves.
Figures 3, 4 and 5 depict the transmission spectra of photonic
quantum well structures (AB)8/(C)*n*/(BA)8. The transmission was

(a)

(b)

(c)

(d)

(e)

(f)

Figure 5. Transmission of PQW structure (AB)8C5(BA)8, for TE

mode with angle of incidence (a) *θ* = 0*◦*, (b) *θ* = 45*◦*, (c) *θ* = 80*◦*
and for TM mode with angle of incidence (d) *θ*= 0*◦*_{, (e)} _{θ}_{= 45}*◦*_{, (f)}

*θ*= 80*◦*_{.}

figures that no waves can transmit in the low-frequency range while
nearly all the high-frequency waves can pass through for the TE modes.
Contrasting the TM modes with the TE modes, the only discrimination
is that two striking TM defect modes come out in the low-frequency
range which gradually shifts left with increasing number of defect layers
(*n*). It is similar to results obtained for multilayer photonic structure
with increase in the thickness of defect layer [11]. This device can be
used to filter a narrow wavelength or frequency out of the incident
radiation within the PBG region.

In the case of normal incidence (*θ* = 0*◦*_{), both TE and TM modes}
have the same values, so the filter channel modes are also at same
wavelength. While at the other (non-zero) angle of incidence, both TE
and TM modes present separate patterns of transmission spectra and
band gap region as shown in above figures. As the angle of incidence
increases, the filter channel mode moves towards the lower wavelength
or higher frequency range with the PBG region.

As the number of layers C*n*increases, the number of filter channels
also increases, as shown in Figures 4 and 5. As the number of defect
layers C*n* increases from 1 to 5, the corresponding resonant frequency
modes will also be increased, leading to an increase in the number of
filter channels into the PBG region. These multi-channel filters can be
tuned with the angle of incidence of light along with the PBG region
to obtain the desired result. With the PQW structures, by properly
choosing the geometric and dielectric parameters, a large number of
multi-channel filter mode can be achieved, which may have potential
application as narrow band filters. For instance, this structure can be
used as a multi-channel filter that can transmit multi wavelength or
frequency singles with a single device in infrared region.

4. CONCLUSION

These results show that the PQW structures have been used to achieve multi-channel filter modes in the photonic band gap region. The PQW structure can be used to design multi-channel filter of 1-D PQW structure. These multi-channel filters can also be tuned with the angle of incidence of light. Also, such structures can be used for the design of optical devices like multi-channel filter, resonators, etc.

REFERENCES

1. Yablonovitch, E., “Inhibited spontaneous emission in solid-state
physics and electronics,” *Phys. Rev. Lett.*, Vol. 58, 2059–2062,
1987.

2. John, S., “Strong localization of photons in certain disordered
dielectric superlattices,” *Phys. Rev. Lett.*, Vol. 58, 2486–2489,
1987.

3. Dowling, J. P., “Mirror on the wall: You’re omnidirectional after
all?” *Science*, Vol. 282, 1841–1843, 1998.

5. Chigrin, D. N., A. V. Lavrinenko, D. A. Yarotsky, and
S. V. Gaponenko, “Observation of total omnidirectional reflection
from a one-dimensional dielectric lattice,”*Appl. Phys. A: Mater.*
*Sci. Process.*, Vol. 68, 25–28, 1999.

6. Fink, Y., J. N. Winn, S. Fan, C. Chen, J. Michel, J. D. Joannopou-los, and E. L. Thomas, “A dielectric omnidirectional reflector,”

*Science*, Vol. 282, 1679–1682, 1998.

7. Lusk, D., I. Abdulhalim, and F. Placido, “Omnidirectional
reflection from Fibonacci quasi-periodic one-dimensional photonic
crystal,”*Opt. Commun.*, Vol. 198, 273–279, 2001.

8. Ibanescu, M., Y. Fink, S. Fan, E. L. Thomas, and
J. D. Joannopoulos, “An all-dielectric coaxial waveguide,”
*Sci-ence*, Vol. 289, 415–418, 2000.

9. Srivastava, S. K. and S. P. Ojha, “Omnidirectional reflection bands
in one-dimensional photonic crystal structure using fluorescence
films,” *Progress In Electromagnetics Research*, Vol. 74, 181–194,
2007.

10. Srivastava, R., S. Pati, and S. P. Ojha, “Enhancement of omnidirectional reflection in photonic crystal heterostructures,”

*Progress In Electromagnetics Research B*, Vol. 1, 197–208, 2008.
11. Bhargava, A. and B. Suthar, “Localized modes in chalcogenide

photonic multilayers with As-S-Se defect layer,” *Chalcogenide*
*Letters*, Vol. 6, No. 10, 529–533, 2009.

12. Villar, I. D., I. R. Mat´ıas, F. J. Arregui, and R. O. Claus,
“Analysis of one-dimensional photonic band gap structures with
a liquid crystal defect towards development of fiber-optic tunable
wavelength filters,” *Optics Express*, Vol. 11, 430–36, 2003.

13. Zhang, Y. and B. Y. Gu, “Aperiodic photonic quantum-well
structures for multiple channeled filtering at arbitrary preassigned
frequencies,”*Optics Express*, Vol. 12, 5910–15, 2004.

14. Xiao, F., B. Juswardy, and K. Alameh, “Tunable photonic
microwave filters based on opto-VLSI processors,” *IEEE*
*Photonics Technology Letters*, Vol. 21, 751–53, 2009.

15. Yang, W. X., J. M. Hou, and R. K. Lee, “Ultraslow bright and
dark solitons in semiconductor quantum wells,” *Phys. Rev. A*,
Vol. 77, (033838)1–7, 2008.

17. Schindler, C. and R. Zimmermann, “Analysis of the
exciton-exciton interaction in semiconductor quantum wells,” *Phys. Rev.*
*B*, Vol. 78, 045313, 2008.

18. Politano, A. and G. Chiarello, “Collective electronic excitations in
systems exhibiting quantum well states,”*Surf. Rev. Lett.*, Vol. 16,
171–190, 2009.

19. Politano, A. and G. Chiarello, “Enhancement of hydrolysis in
alkali ultrathin layers on metal substrates in the presence of
electron confinement,”*Chem. Phys. Lett.*, Vol. 494, 84–87, 2010.
20. Politano, A., R. G. Agostino, E. Colavita, V. Formoso, and

G. Chiarello, “Purely quadratic dispersion of surface plasmon in
Ag/Ni(111): The influence of electron confinement,”*Phys. Status*
*Solidi Rapid Res. Lett. (RRL)*, Vol. 2, 86–88, 2008.

21. Zhang, C., F. Qiao, J. Wan, and J. Zi, “Enlargement of
nontransmission frequency range in photonic crystals by using
multiple heterostructures,” *J. Appl. Phys.*, Vol. 87, 3174–3176,
2000.

22. Qiao, F., C. Zhang, J. Wan, and J. Zi, “Photonic quantum-well
structures: Multiple channeled filtering phenomena,”*Appl. Phys.*
*Lett.*, Vol. 77, 3698–3700, 2000.

23. Xiang, Y., X. Dai, S. Wen, and D. Fan, “Omnidirectional and
multiple-channeled high-quality filters of photonic
heterostruc-tures containing single-negative materials,” *J. Opt. Soc. Am. A*,
Vol. 24, A28–A32, 2007.

24. Chen, Y. H., “Frequency response of resonance modes in
heterostructures composed of single-negative materials,” *J. Opt.*
*Soc. Am. B*, Vol. 25, 1794–1799, 2008.

25. Yeh, P., *Optical Waves in Layered Media*, John Wiley and Sons,
New York, 1988.